#------------------------------------------------------------------------------
#$Date: 2025-07-01 13:44:25 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1119 $
#$URL: svn://crystallography.net/testcod/cif/2/00/00/2000016.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2000016
loop_
_publ_author_name
'Strange, Nicholas A.'
'Bell, Robert T.'
'Park, James Eujin'
'Stone, Kevin H.'
'Coker, Eric N.'
'Ginley, David S.'
_publ_section_title
;
 Formation of Ba3Nb0.75Mn2.25O9-6H during thermochemical reduction of
 Ba4NbMn3O12-12R
;
_journal_issue                   5
_journal_name_full
'Acta Crystallographica Section E Crystallographic Communications'
_journal_page_first              469
_journal_page_last               473
_journal_paper_doi               10.1107/S2056989023003213
_journal_volume                  79
_journal_year                    2023
_chemical_formula_sum            'Ba6 Mn4.5 Nb1.5 O18'
_chemical_formula_weight         1498.53199
_space_group_crystal_system      hexagonal
_space_group_IT_number           194
_space_group_name_Hall           '-P 6c 2c'
_space_group_name_H-M_alt        'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   5.743123(13)
_cell_length_b                   5.743123(13)
_cell_length_c                   14.09930(5)
_cell_measurement_reflns_used    1932
_cell_measurement_temperature    300
_cell_measurement_theta_max      41.75
_cell_measurement_theta_min      2.5
_cell_volume                     402.7397(19)
_diffrn_ambient_temperature      300
_diffrn_measured_fraction_theta_full 213
_diffrn_measurement_device_type  SSRL_beamline_2-1
_diffrn_radiation_wavelength     0.729276500
_exptl_absorpt_coefficient_mu    20.118
_exptl_crystal_density_diffrn    6.17861(4)
_pd_block_diffractogram_id       Bell_BNM_1350_0ppmO2_scan1
_pd_block_id                     6H-barium_niobium_manganese_oxide
_pd_phase_name                   6H-Ba3Nb0.75Mn2.25O9
_cod_data_source_file            wm5677sup2.txt
_cod_data_source_block           6H-barium_niobium_manganese_oxide
_cod_original_cell_volume        402.740(2)
_cod_original_sg_symbol_H-M      P63/mmc
_cod_original_formula_sum        Ba6Nb1.5Mn4.5O18
_cod_database_code               2000016
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z '
2 '-x, -x+y, z+1/2 '
3 '-x, -y, -z '
4 '-x, -y, z+1/2 '
5 '-x+y, -x, -z+1/2 '
6 '-x+y, -x, z '
7 '-x+y, y, -z+1/2 '
8 '-x+y, y, z '
9 '-y, -x, -z+1/2 '
10 '-y, -x, z '
11 '-y, x-y, -z+1/2 '
12 '-y, x-y, z '
13 'y, -x+y, -z '
14 'y, -x+y, z+1/2 '
15 'y, x, -z '
16 'y, x, z+1/2 '
17 'x-y, -y, -z '
18 'x-y, -y, z+1/2 '
19 'x-y, x, -z '
20 'x-y, x, z+1/2 '
21 'x, y, -z+1/2 '
22 '-x, -x+y, -z '
23 'x, x-y, -z+1/2 '
24 'x, x-y, z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_site_symmetry_multiplicity
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Ba1 Ba+2 2 0 0 0.25 1 0.93(3)
Ba2 Ba+2 4 0.3333333 0.6666667 0.08847(3) 1 0.93(3)
Mn1 Mn+4 4 0.3333333 0.6666667 0.65603(7) 1 0.44(3)
Nb1 Nb+5 2 0 0 0 0.75 0.44(3)
Mn2 Mn+3 2 0 0 0 0.25 0.44(3)
O1 O-2 6 0.5215(4) 1.0430(8) 0.25 1 1.68(5)
O2 O-2 12 0.1690(3) 0.3380(6) 0.58332(19) 1 1.68(5)
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
O1 Ba1 O1 51.48(16) 9_665 1_555 1_445
O1 Ba1 O1 171.48(16) 9_655 1_555 9_665
O1 Ba1 O1 120.000 9_655 1_555 1_445
O1 Ba1 O1 68.52(16) 1_545 1_555 9_655
O1 Ba1 O1 120.000 1_545 1_555 9_665
O1 Ba1 O1 171.48(16) 1_545 1_555 1_445
O1 Ba1 O1 51.48(16) 5_565 1_555 1_545
O1 Ba1 O1 120.000 5_565 1_555 9_655
O1 Ba1 O1 68.52(16) 5_565 1_555 9_665
O1 Ba1 O1 120.000 5_565 1_555 1_445
O1 Ba1 O1 171.48(16) 5_455 1_555 5_565
O1 Ba1 O1 120.000 5_455 1_555 1_545
O1 Ba1 O1 51.48(16) 5_455 1_555 9_655
O1 Ba1 O1 120.000 5_455 1_555 9_665
O1 Ba1 O1 68.52(16) 5_455 1_555 1_445
O2 Ba1 O1 118.74(5) 14_554 1_555 5_455
O2 Ba1 O1 58.39(5) 14_554 1_555 5_565
O2 Ba1 O1 58.39(5) 14_554 1_555 1_545
O2 Ba1 O1 92.48(5) 14_554 1_555 9_655
O2 Ba1 O1 92.48(5) 14_554 1_555 9_665
O2 Ba1 O1 118.74(5) 14_554 1_555 1_445
O2 Ba1 O2 146.18(5) 3_556 1_555 14_554
O2 Ba1 O1 58.39(5) 3_556 1_555 5_455
O2 Ba1 O1 118.74(5) 3_556 1_555 5_565
O2 Ba1 O1 92.48(5) 3_556 1_555 1_545
O2 Ba1 O1 58.39(5) 3_556 1_555 9_655
O2 Ba1 O1 118.74(5) 3_556 1_555 9_665
O2 Ba1 O1 92.48(5) 3_556 1_555 1_445
O2 Ba1 O2 146.18(5) 2_554 1_555 3_556
O2 Ba1 O2 60.51(9) 2_554 1_555 14_554
O2 Ba1 O1 92.48(5) 2_554 1_555 5_455
O2 Ba1 O1 92.48(5) 2_554 1_555 5_565
O2 Ba1 O1 118.74(5) 2_554 1_555 1_545
O2 Ba1 O1 118.74(5) 2_554 1_555 9_655
O2 Ba1 O1 58.39(5) 2_554 1_555 9_665
O2 Ba1 O1 58.39(5) 2_554 1_555 1_445
O2 Ba1 O2 108.85(12) 19_556 1_555 2_554
O2 Ba1 O2 60.51(9) 19_556 1_555 3_556
O2 Ba1 O2 146.18(5) 19_556 1_555 14_554
O2 Ba1 O1 92.48(5) 19_556 1_555 5_455
O2 Ba1 O1 92.48(5) 19_556 1_555 5_565
O2 Ba1 O1 118.74(5) 19_556 1_555 1_545
O2 Ba1 O1 118.74(5) 19_556 1_555 9_655
O2 Ba1 O1 58.39(5) 19_556 1_555 9_665
O2 Ba1 O1 58.39(5) 19_556 1_555 1_445
O2 Ba1 O2 146.18(5) 4_554 1_555 19_556
O2 Ba1 O2 60.51(9) 4_554 1_555 2_554
O2 Ba1 O2 108.85(12) 4_554 1_555 3_556
O2 Ba1 O2 60.51(9) 4_554 1_555 14_554
O2 Ba1 O1 58.39(5) 4_554 1_555 5_455
O2 Ba1 O1 118.74(5) 4_554 1_555 5_565
O2 Ba1 O1 92.48(5) 4_554 1_555 1_545
O2 Ba1 O1 58.39(5) 4_554 1_555 9_655
O2 Ba1 O1 118.74(5) 4_554 1_555 9_665
O2 Ba1 O1 92.48(5) 4_554 1_555 1_445
O2 Ba1 O2 146.18(5) 13_556 1_555 4_554
O2 Ba1 O2 60.51(9) 13_556 1_555 19_556
O2 Ba1 O2 146.18(5) 13_556 1_555 2_554
O2 Ba1 O2 60.51(9) 13_556 1_555 3_556
O2 Ba1 O2 108.85(12) 13_556 1_555 14_554
O2 Ba1 O1 118.74(5) 13_556 1_555 5_455
O2 Ba1 O1 58.39(5) 13_556 1_555 5_565
O2 Ba1 O1 58.39(5) 13_556 1_555 1_545
O2 Ba1 O1 92.48(5) 13_556 1_555 9_655
O2 Ba1 O1 92.48(5) 13_556 1_555 9_665
O2 Ba1 O1 118.74(5) 13_556 1_555 1_445
O2 Ba2 O2 119.937(2) 14_564 1_555 4_664
O2 Ba2 O2 176.96(11) 14_554 1_555 14_564
O2 Ba2 O2 59.06(13) 14_554 1_555 4_664
O2 Ba2 O2 119.937(2) 4_564 1_555 14_554
O2 Ba2 O2 60.90(13) 4_564 1_555 14_564
O2 Ba2 O2 176.96(11) 4_564 1_555 4_664
O2 Ba2 O2 119.937(2) 2_664 1_555 4_564
O2 Ba2 O2 119.937(2) 2_664 1_555 14_554
O2 Ba2 O2 59.06(13) 2_664 1_555 14_564
O2 Ba2 O2 60.90(13) 2_664 1_555 4_664
O2 Ba2 O2 176.96(11) 2_554 1_555 2_664
O2 Ba2 O2 59.06(13) 2_554 1_555 4_564
O2 Ba2 O2 60.90(13) 2_554 1_555 14_554
O2 Ba2 O2 119.937(2) 2_554 1_555 14_564
O2 Ba2 O2 119.937(2) 2_554 1_555 4_664
O2 Ba2 O2 117.75(4) 9_665 1_555 2_554
O2 Ba2 O2 59.80(10) 9_665 1_555 2_664
O2 Ba2 O2 117.75(4) 9_665 1_555 4_564
O2 Ba2 O2 88.54(6) 9_665 1_555 14_554
O2 Ba2 O2 88.54(6) 9_665 1_555 14_564
O2 Ba2 O2 59.80(10) 9_665 1_555 4_664
O2 Ba2 O2 57.96(10) 5_565 1_555 9_665
O2 Ba2 O2 88.54(6) 5_565 1_555 2_554
O2 Ba2 O2 88.54(6) 5_565 1_555 2_664
O2 Ba2 O2 59.80(10) 5_565 1_555 4_564
O2 Ba2 O2 117.75(4) 5_565 1_555 14_554
O2 Ba2 O2 59.80(10) 5_565 1_555 14_564
O2 Ba2 O2 117.75(4) 5_565 1_555 4_664
O2 Ba2 O2 57.96(10) 7_555 1_555 5_565
O2 Ba2 O2 57.96(10) 7_555 1_555 9_665
O2 Ba2 O2 59.80(10) 7_555 1_555 2_554
O2 Ba2 O2 117.75(4) 7_555 1_555 2_664
O2 Ba2 O2 88.54(6) 7_555 1_555 4_564
O2 Ba2 O2 59.80(10) 7_555 1_555 14_554
O2 Ba2 O2 117.75(4) 7_555 1_555 14_564
O2 Ba2 O2 88.54(6) 7_555 1_555 4_664
O1 Ba2 O2 117.56(7) 9_665 1_555 7_555
O1 Ba2 O2 117.56(7) 9_665 1_555 5_565
O1 Ba2 O2 174.60(8) 9_665 1_555 9_665
O1 Ba2 O2 57.81(7) 9_665 1_555 2_554
O1 Ba2 O2 124.52(7) 9_665 1_555 2_664
O1 Ba2 O2 57.81(7) 9_665 1_555 4_564
O1 Ba2 O2 91.41(6) 9_665 1_555 14_554
O1 Ba2 O2 91.41(6) 9_665 1_555 14_564
O1 Ba2 O2 124.52(7) 9_665 1_555 4_664
O1 Ba2 O1 66.72(10) 5_565 1_555 9_665
O1 Ba2 O2 117.56(7) 5_565 1_555 7_555
O1 Ba2 O2 174.60(8) 5_565 1_555 5_565
O1 Ba2 O2 117.56(7) 5_565 1_555 9_665
O1 Ba2 O2 91.41(6) 5_565 1_555 2_554
O1 Ba2 O2 91.41(6) 5_565 1_555 2_664
O1 Ba2 O2 124.52(7) 5_565 1_555 4_564
O1 Ba2 O2 57.81(7) 5_565 1_555 14_554
O1 Ba2 O2 124.52(7) 5_565 1_555 14_564
O1 Ba2 O2 57.81(7) 5_565 1_555 4_664
O1 Ba2 O1 66.72(10) 1_555 1_555 5_565
O1 Ba2 O1 66.72(10) 1_555 1_555 9_665
O1 Ba2 O2 174.60(8) 1_555 1_555 7_555
O1 Ba2 O2 117.56(7) 1_555 1_555 5_565
O1 Ba2 O2 117.56(7) 1_555 1_555 9_665
O1 Ba2 O2 124.52(7) 1_555 1_555 2_554
O1 Ba2 O2 57.81(7) 1_555 1_555 2_664
O1 Ba2 O2 91.41(6) 1_555 1_555 4_564
O1 Ba2 O2 124.52(7) 1_555 1_555 14_554
O1 Ba2 O2 57.81(7) 1_555 1_555 14_564
O1 Ba2 O2 91.41(6) 1_555 1_555 4_664
O2 Mn1 O2 94.39(12) 10_665 1_555 6_565
O2 Mn1 O2 94.39(12) 1_555 1_555 10_665
O2 Mn1 O2 94.39(12) 1_555 1_555 6_565
O1 Mn1 O2 92.70(9) 13_456 1_555 1_555
O1 Mn1 O2 169.55(13) 13_456 1_555 10_665
O1 Mn1 O2 92.70(9) 13_456 1_555 6_565
O1 Mn1 O1 79.30(14) 2_655 1_555 13_456
O1 Mn1 O2 92.70(9) 2_655 1_555 1_555
O1 Mn1 O2 92.70(9) 2_655 1_555 10_665
O1 Mn1 O2 169.55(13) 2_655 1_555 6_565
O1 Mn1 O1 79.30(14) 3_676 1_555 2_655
O1 Mn1 O1 79.30(14) 3_676 1_555 13_456
O1 Mn1 O2 169.55(13) 3_676 1_555 1_555
O1 Mn1 O2 92.70(9) 3_676 1_555 10_665
O1 Mn1 O2 92.70(9) 3_676 1_555 6_565
Mn1 Mn1 O1 47.46(9) 5_566 1_555 3_676
Mn1 Mn1 O1 47.46(9) 5_566 1_555 2_655
Mn1 Mn1 O1 47.46(9) 5_566 1_555 13_456
Mn1 Mn1 O2 122.09(9) 5_566 1_555 1_555
Mn1 Mn1 O2 122.09(9) 5_566 1_555 10_665
Mn1 Mn1 O2 122.09(9) 5_566 1_555 6_565
O2 Nb1 Mn2 . 7_555 1_555 1_555
O2 Nb1 O2 90.45(11) 5_555 1_555 7_555
O2 Nb1 Mn2 . 5_555 1_555 1_555
O2 Nb1 O2 179.99999879(6) 2_554 1_555 5_555
O2 Nb1 O2 89.55(11) 2_554 1_555 7_555
O2 Nb1 Mn2 . 2_554 1_555 1_555
O2 Nb1 O2 90.45(11) 4_554 1_555 2_554
O2 Nb1 O2 89.55(11) 4_554 1_555 5_555
O2 Nb1 O2 180.00000000(3) 4_554 1_555 7_555
O2 Nb1 Mn2 . 4_554 1_555 1_555
O2 Nb1 O2 89.55(11) 9_555 1_555 4_554
O2 Nb1 O2 89.55(11) 9_555 1_555 2_554
O2 Nb1 O2 90.45(11) 9_555 1_555 5_555
O2 Nb1 O2 90.45(11) 9_555 1_555 7_555
O2 Nb1 Mn2 . 9_555 1_555 1_555
O2 Nb1 O2 180.000 14_554 1_555 9_555
O2 Nb1 O2 90.45(11) 14_554 1_555 4_554
O2 Nb1 O2 90.45(11) 14_554 1_555 2_554
O2 Nb1 O2 89.55(11) 14_554 1_555 5_555
O2 Nb1 O2 89.55(11) 14_554 1_555 7_555
O2 Nb1 Mn2 . 14_554 1_555 1_555
O2 Mn2 Nb1 . 7_555 1_555 1_555
O2 Mn2 O2 90.45(11) 5_555 1_555 7_555
O2 Mn2 Nb1 . 5_555 1_555 1_555
O2 Mn2 O2 179.99999879(6) 2_554 1_555 5_555
O2 Mn2 O2 89.55(11) 2_554 1_555 7_555
O2 Mn2 Nb1 . 2_554 1_555 1_555
O2 Mn2 O2 90.45(11) 4_554 1_555 2_554
O2 Mn2 O2 89.55(11) 4_554 1_555 5_555
O2 Mn2 O2 180.00000000(3) 4_554 1_555 7_555
O2 Mn2 Nb1 . 4_554 1_555 1_555
O2 Mn2 O2 89.55(11) 9_555 1_555 4_554
O2 Mn2 O2 89.55(11) 9_555 1_555 2_554
O2 Mn2 O2 90.45(11) 9_555 1_555 5_555
O2 Mn2 O2 90.45(11) 9_555 1_555 7_555
O2 Mn2 Nb1 . 9_555 1_555 1_555
O2 Mn2 O2 180.000 14_554 1_555 9_555
O2 Mn2 O2 90.45(11) 14_554 1_555 4_554
O2 Mn2 O2 90.45(11) 14_554 1_555 2_554
O2 Mn2 O2 89.55(11) 14_554 1_555 5_555
O2 Mn2 O2 89.55(11) 14_554 1_555 7_555
O2 Mn2 Nb1 . 14_554 1_555 1_555
Mn1 O1 Mn1 85.08(18) 3_676 1_555 2_664
O1 O1 Mn1 50.35(7) 5_575 1_555 3_676
O1 O1 Mn1 50.35(7) 5_575 1_555 2_664
O1 O1 O1 60.000 9_775 1_555 5_575
O1 O1 Mn1 50.35(7) 9_775 1_555 3_676
O1 O1 Mn1 50.35(7) 9_775 1_555 2_664
O2 O1 O1 63.62(8) 2_664 1_555 9_775
O2 O1 O1 93.37(9) 2_664 1_555 5_575
O2 O1 Mn1 113.61(15) 2_664 1_555 3_676
O2 O1 Mn1 43.23(6) 2_664 1_555 2_664
O2 O1 O2 154.27(18) 13_566 1_555 2_664
O2 O1 O1 93.37(9) 13_566 1_555 9_775
O2 O1 O1 63.62(8) 13_566 1_555 5_575
O2 O1 Mn1 43.23(6) 13_566 1_555 3_676
O2 O1 Mn1 113.61(15) 13_566 1_555 2_664
O2 O1 O2 113.25(10) 14_564 1_555 13_566
O2 O1 O2 60.41(12) 14_564 1_555 2_664
O2 O1 O1 93.37(9) 14_564 1_555 9_775
O2 O1 O1 63.62(8) 14_564 1_555 5_575
O2 O1 Mn1 113.61(15) 14_564 1_555 3_676
O2 O1 Mn1 43.23(6) 14_564 1_555 2_664
O2 O1 O2 154.27(18) 19_666 1_555 14_564
O2 O1 O2 60.41(12) 19_666 1_555 13_566
O2 O1 O2 113.25(10) 19_666 1_555 2_664
O2 O1 O1 63.62(8) 19_666 1_555 9_775
O2 O1 O1 93.37(9) 19_666 1_555 5_575
O2 O1 Mn1 43.23(6) 19_666 1_555 3_676
O2 O1 Mn1 113.61(15) 19_666 1_555 2_664
Ba1 O1 O2 60.98(6) 1_665 1_555 19_666
Ba1 O1 O2 121.21(6) 1_665 1_555 14_564
Ba1 O1 O2 121.21(6) 1_665 1_555 13_566
Ba1 O1 O2 60.98(6) 1_665 1_555 2_664
Ba1 O1 O1 64.26(8) 1_665 1_555 9_775
Ba1 O1 O1 124.26(8) 1_665 1_555 5_575
Ba1 O1 Mn1 93.14(5) 1_665 1_555 3_676
Ba1 O1 Mn1 93.14(5) 1_665 1_555 2_664
Ba1 O1 Ba1 171.48(16) 1_565 1_555 1_665
Ba1 O1 O2 121.21(6) 1_565 1_555 19_666
Ba1 O1 O2 60.98(6) 1_565 1_555 14_564
Ba1 O1 O2 60.98(6) 1_565 1_555 13_566
Ba1 O1 O2 121.21(6) 1_565 1_555 2_664
Ba1 O1 O1 124.26(8) 1_565 1_555 9_775
Ba1 O1 O1 64.26(8) 1_565 1_555 5_575
Ba1 O1 Mn1 93.14(5) 1_565 1_555 3_676
Ba1 O1 Mn1 93.14(5) 1_565 1_555 2_664
Ba2 O1 Ba1 87.30(6) 5_565 1_555 1_565
Ba2 O1 Ba1 87.30(6) 5_565 1_555 1_665
Ba2 O1 O2 59.75(4) 5_565 1_555 19_666
Ba2 O1 O2 141.86(12) 5_565 1_555 14_564
Ba2 O1 O2 59.75(4) 5_565 1_555 13_566
Ba2 O1 O2 141.86(12) 5_565 1_555 2_664
Ba2 O1 O1 123.36(5) 5_565 1_555 9_775
Ba2 O1 O1 123.36(5) 5_565 1_555 5_575
Ba2 O1 Mn1 86.88(3) 5_565 1_555 3_676
Ba2 O1 Mn1 171.96(15) 5_565 1_555 2_664
Ba2 O1 Ba2 101.17(12) 1_555 1_555 5_565
Ba2 O1 Ba1 87.30(6) 1_555 1_555 1_565
Ba2 O1 Ba1 87.30(6) 1_555 1_555 1_665
Ba2 O1 O2 141.86(12) 1_555 1_555 19_666
Ba2 O1 O2 59.75(4) 1_555 1_555 14_564
Ba2 O1 O2 141.86(12) 1_555 1_555 13_566
Ba2 O1 O2 59.75(4) 1_555 1_555 2_664
Ba2 O1 O1 123.36(5) 1_555 1_555 9_775
Ba2 O1 O1 123.36(5) 1_555 1_555 5_575
Ba2 O1 Mn1 171.96(15) 1_555 1_555 3_676
Ba2 O1 Mn1 86.88(3) 1_555 1_555 2_664
Mn2 O2 Mn1 177.14(13) 2_555 1_555 1_555
Nb1 O2 Mn2 0.000 2_555 1_555 2_555
Nb1 O2 Mn1 177.14(13) 2_555 1_555 1_555
O1 O2 Nb1 138.09(13) 13_456 1_555 2_555
O1 O2 Mn2 138.09(13) 13_456 1_555 2_555
O1 O2 Mn1 44.07(9) 13_456 1_555 1_555
O1 O2 O1 52.76(15) 2_655 1_555 13_456
O1 O2 Nb1 138.09(13) 2_655 1_555 2_555
O1 O2 Mn2 138.09(13) 2_655 1_555 2_555
O1 O2 Mn1 44.07(9) 2_655 1_555 1_555
O2 O2 O1 86.63(9) 6_565 1_555 2_655
O2 O2 O1 59.80(6) 6_565 1_555 13_456
O2 O2 Nb1 135.22(5) 6_565 1_555 2_555
O2 O2 Mn2 135.22(5) 6_565 1_555 2_555
O2 O2 Mn1 42.80(6) 6_565 1_555 1_555
O2 O2 O2 60.000 10_665 1_555 6_565
O2 O2 O1 59.80(6) 10_665 1_555 2_655
O2 O2 O1 86.63(9) 10_665 1_555 13_456
O2 O2 Nb1 135.22(5) 10_665 1_555 2_555
O2 O2 Mn2 135.22(5) 10_665 1_555 2_555
O2 O2 Mn1 42.80(6) 10_665 1_555 1_555
Ba2 O2 O2 120.45(6) 2_555 1_555 10_665
Ba2 O2 O2 60.47(6) 2_555 1_555 6_565
Ba2 O2 O1 115.19(11) 2_555 1_555 2_655
Ba2 O2 O1 62.44(8) 2_555 1_555 13_456
Ba2 O2 Nb1 90.45(6) 2_555 1_555 2_555
Ba2 O2 Mn2 90.45(6) 2_555 1_555 2_555
Ba2 O2 Mn1 89.62(6) 2_555 1_555 1_555
Ba2 O2 Ba2 176.96(11) 2_655 1_555 2_555
Ba2 O2 O2 60.47(6) 2_655 1_555 10_665
Ba2 O2 O2 120.45(6) 2_655 1_555 6_565
Ba2 O2 O1 62.44(8) 2_655 1_555 2_655
Ba2 O2 O1 115.19(11) 2_655 1_555 13_456
Ba2 O2 Nb1 90.45(6) 2_655 1_555 2_555
Ba2 O2 Mn2 90.45(6) 2_655 1_555 2_555
Ba2 O2 Mn1 89.62(6) 2_655 1_555 1_555
O2 O2 Ba2 60.95(6) 13_556 1_555 2_655
O2 O2 Ba2 121.46(10) 13_556 1_555 2_555
O2 O2 O2 90.000 13_556 1_555 10_665
O2 O2 O2 120.26(6) 13_556 1_555 6_565
O2 O2 O1 123.34(9) 13_556 1_555 2_655
O2 O2 O1 175.89(9) 13_556 1_555 13_456
O2 O2 Nb1 45.22(5) 13_556 1_555 2_555
O2 O2 Mn2 45.22(5) 13_556 1_555 2_555
O2 O2 Mn1 132.73(7) 13_556 1_555 1_555
O2 O2 O2 60.52(12) 19_556 1_555 13_556
O2 O2 Ba2 121.46(10) 19_556 1_555 2_655
O2 O2 Ba2 60.95(6) 19_556 1_555 2_555
O2 O2 O2 120.26(6) 19_556 1_555 10_665
O2 O2 O2 90.000 19_556 1_555 6_565
O2 O2 O1 175.89(9) 19_556 1_555 2_655
O2 O2 O1 123.34(9) 19_556 1_555 13_456
O2 O2 Nb1 45.22(5) 19_556 1_555 2_555
O2 O2 Mn2 45.22(5) 19_556 1_555 2_555
O2 O2 Mn1 132.73(7) 19_556 1_555 1_555
Ba1 O2 O2 119.49(8) 2_555 1_555 19_556
Ba1 O2 O2 119.49(8) 2_555 1_555 13_556
Ba1 O2 Ba2 88.55(6) 2_555 1_555 2_655
Ba1 O2 Ba2 88.55(6) 2_555 1_555 2_555
Ba1 O2 O2 120.25(5) 2_555 1_555 10_665
Ba1 O2 O2 120.25(5) 2_555 1_555 6_565
Ba1 O2 O1 60.63(6) 2_555 1_555 2_655
Ba1 O2 O1 60.63(6) 2_555 1_555 13_456
Ba1 O2 Nb1 89.37(10) 2_555 1_555 2_555
Ba1 O2 Mn2 89.37(10) 2_555 1_555 2_555
Ba1 O2 Mn1 93.48(10) 2_555 1_555 1_555
O2 O2 Ba1 59.75(5) 6_555 1_555 2_555
O2 O2 O2 90.000 6_555 1_555 19_556
O2 O2 O2 59.74(6) 6_555 1_555 13_556
O2 O2 Ba2 59.55(6) 6_555 1_555 2_655
O2 O2 Ba2 119.53(6) 6_555 1_555 2_555
O2 O2 O2 120.000 6_555 1_555 10_665
O2 O2 O2 180.00000000(3) 6_555 1_555 6_565
O2 O2 O1 93.37(9) 6_555 1_555 2_655
O2 O2 O1 120.20(6) 6_555 1_555 13_456
O2 O2 Nb1 44.78(5) 6_555 1_555 2_555
O2 O2 Mn2 44.78(5) 6_555 1_555 2_555
O2 O2 Mn1 137.20(6) 6_555 1_555 1_555
O2 O2 O2 60.000 10_555 1_555 6_555
O2 O2 Ba1 59.75(5) 10_555 1_555 2_555
O2 O2 O2 59.74(6) 10_555 1_555 19_556
O2 O2 O2 90.000 10_555 1_555 13_556
O2 O2 Ba2 119.53(6) 10_555 1_555 2_655
O2 O2 Ba2 59.55(6) 10_555 1_555 2_555
O2 O2 O2 180.00000000(3) 10_555 1_555 10_665
O2 O2 O2 120.000 10_555 1_555 6_565
O2 O2 O1 120.20(6) 10_555 1_555 2_655
O2 O2 O1 93.37(9) 10_555 1_555 13_456
O2 O2 Nb1 44.78(5) 10_555 1_555 2_555
O2 O2 Mn2 44.78(5) 10_555 1_555 2_555
O2 O2 Mn1 137.20(6) 10_555 1_555 1_555
Ba2 O2 O2 118.98(5) 5_565 1_555 10_555
Ba2 O2 O2 118.98(5) 5_565 1_555 6_555
Ba2 O2 Ba1 178.44(12) 5_565 1_555 2_555
Ba2 O2 O2 59.25(7) 5_565 1_555 19_556
Ba2 O2 O2 59.25(7) 5_565 1_555 13_556
Ba2 O2 Ba2 91.46(6) 5_565 1_555 2_655
Ba2 O2 Ba2 91.46(6) 5_565 1_555 2_555
Ba2 O2 O2 61.02(5) 5_565 1_555 10_665
Ba2 O2 O2 61.02(5) 5_565 1_555 6_565
Ba2 O2 O1 120.71(10) 5_565 1_555 2_655
Ba2 O2 O1 120.71(10) 5_565 1_555 13_456
Ba2 O2 Nb1 89.07(9) 5_565 1_555 2_555
Ba2 O2 Mn2 89.07(9) 5_565 1_555 2_555
Ba2 O2 Mn1 88.07(12) 5_565 1_555 1_555
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
Ba1 O1 2.8795(4) 1_555 1_445
Ba1 O1 2.8795(4) 1_555 9_665
Ba1 O1 2.8795(4) 1_555 9_655
Ba1 O1 2.8795(4) 1_555 1_545
Ba1 O1 2.8795(4) 1_555 5_565
Ba1 O1 2.8795(4) 1_555 5_455
Ba1 O2 2.889(3) 1_555 14_554
Ba1 O2 2.889(3) 1_555 3_556
Ba1 O2 2.889(3) 1_555 2_554
Ba1 O2 2.889(3) 1_555 19_556
Ba1 O2 2.889(3) 1_555 4_554
Ba1 O2 2.889(3) 1_555 13_556
Ba2 O2 2.87257(12) 1_555 4_664
Ba2 O2 2.87257(12) 1_555 14_564
Ba2 O2 2.87257(12) 1_555 14_554
Ba2 O2 2.87257(12) 1_555 4_564
Ba2 O2 2.87257(12) 1_555 2_664
Ba2 O2 2.87257(12) 1_555 2_554
Ba2 O2 2.922(3) 1_555 9_665
Ba2 O2 2.922(3) 1_555 5_565
Ba2 O2 2.922(3) 1_555 7_555
Ba2 O1 2.948(3) 1_555 9_665
Ba2 O1 2.948(3) 1_555 5_565
Ba2 O1 2.948(3) 1_555 1_555
Mn1 O2 1.930(3) 1_555 6_565
Mn1 O2 1.930(3) 1_555 10_665
Mn1 O2 1.930(3) 1_555 1_555
Mn1 O1 1.960(3) 1_555 13_456
Mn1 O1 1.960(3) 1_555 2_655
Mn1 O1 1.960(3) 1_555 3_676
Mn1 Mn1 2.6498(18) 1_555 5_566
Nb1 Mn2 0.00000 1_555 1_555
Nb1 O2 2.051(3) 1_555 7_555
Nb1 O2 2.051(3) 1_555 5_555
Nb1 O2 2.051(3) 1_555 2_554
Nb1 O2 2.051(3) 1_555 4_554
Nb1 O2 2.051(3) 1_555 9_555
Nb1 O2 2.051(3) 1_555 14_554
Mn2 Nb1 0.00000 1_555 1_555
Mn2 O2 2.051(3) 1_555 7_555
Mn2 O2 2.051(3) 1_555 5_555
Mn2 O2 2.051(3) 1_555 2_554
Mn2 O2 2.051(3) 1_555 4_554
Mn2 O2 2.051(3) 1_555 9_555
Mn2 O2 2.051(3) 1_555 14_554
O1 Mn1 1.960(3) 1_555 2_664
O1 Mn1 1.960(3) 1_555 3_676
O1 O1 2.501(7) 1_555 5_575
O1 O1 2.501(7) 1_555 9_775
O1 O2 2.814(3) 1_555 2_664
O1 O2 2.814(3) 1_555 13_566
O1 O2 2.814(3) 1_555 14_564
O1 O2 2.814(3) 1_555 19_666
O1 Ba1 2.8795(4) 1_555 1_665
O1 Ba1 2.8795(4) 1_555 1_565
O1 Ba2 2.948(3) 1_555 5_565
O1 Ba2 2.948(3) 1_555 1_555
O2 Mn1 1.930(3) 1_555 1_555
O2 Mn2 2.051(3) 1_555 2_555
O2 Nb1 2.051(3) 1_555 2_555
O2 O1 2.814(3) 1_555 13_456
O2 O1 2.814(3) 1_555 2_655
O2 O2 2.832(5) 1_555 6_565
O2 O2 2.832(5) 1_555 10_665
O2 Ba2 2.87257(12) 1_555 2_555
O2 Ba2 2.87257(12) 1_555 2_655
O2 O2 2.889(5) 1_555 13_556
O2 O2 2.889(5) 1_555 19_556
O2 Ba1 2.889(3) 1_555 2_555
O2 O2 2.912(5) 1_555 6_555
O2 O2 2.912(5) 1_555 10_555
O2 Ba2 2.922(3) 1_555 5_565
